Effect of Fiber Orientation on Mechanical Properties of
Woven Bamboo/E-Glass Fiber Reinforced Epoxy
VENKATESHA B K,
Ph.D Scholar, Dept. of Mechanical Engg, University Visvesvaraya College of Engg, Bangalore/Asst. Professor, School of Mechanical
Engg, REVA University, Bangalore. E-mail: firstname.lastname@example.org
Dr. R. SARAVANAN,
Asst. Professor, Dept. of Mechanical Engineering, University Visvesvaraya College of Engineering, Bangalore
Dr. D SARAVANA BAVAN,
Associate Professor, Department of Mechanical Engg, Dayananada Sagar
Now days there has been a greater importance towards development of natural fiber reinforced polymer composites because these are environmentally friendly and cost effective to synthetic fiber reinforced composites. But, natural fiber reinforced composites are the poor resistance to absorption of moisture. Due to this problem, a natural fiber may be combined with a synthetic fiber with the same matrix material so as to achieve the best advantage in enhancement of their properties. In this connection, hybrid composite materials of natural and man-made fibers reinforced polymer composites are essential for current demands. This paper deals with investigating the effect of fiber orientation on mechanical properties of bi-directional Bamboo and E-Glass fiber reinforced epoxy hybrid composites. This hybrid samples was prepared at different
fiber orientations such as 150, 300, and 600. The hand lay-up method is adopted to prepared the samples. The mechanical
properties such as tensile strength, flexural strength, and inter-laminar shear strength is evaluated experimentally according
to ASTM standards. The conclusions drawn on the basis of the experimental results are discussed and composite with 150
fiber orientation shows better tensile strength compared with other fiber orientations. Similar observations are also presented for other mechanical properties of the composites such as flexural strength, and inter-laminar shear strength. The morphology of testing tensile surfaces is examined using scanning electron microscopy (SEM), and propable fracture mechanisms are identified clearly.
Keywords - Bamoo fiber, hybrid composites, fiber orientation, mechanical properties, hand lay-up method,
ASTM standards, SEM.
To obtain the favorable material properties for a particular application, it is important to know how the material performance changes with the fiber orientation  under given loading conditions. D. Dash, et.al.  studied the mechanical properties of jute fiber and bamboo fiber reinforced epoxy hybrid composites. Hand lay-up technique was used for fabrication of the composite specimens with fiber orientation (0/900, 15/-750, 30/-600, and 45/-450). The results concluded that the fiber orientation of 0/900 provides higher strength and stiffness than other fiber orientations. S. Biswas, et. al. investigated the effect of fiber loading and fiber orientation on mechanical and erosion behavior of glass fiber reinforced epoxy composites. The results revealed the composite with 300 fiber orientation showed better micro hardness compared with other fiber orientations and 600 fiber orientation showed superior tensile modulus and impact energy, where as tensile strength, and flexural strength, showed better results in 150, 300, and 150 fiber orientation with the increase in fiber loading. Vijaya Ramnath B, et.al. evaluated the mechanical behaviour of a jute-flax based glass fiber reinforced composite. The results revealed that the hybrid composite exhibited good mechanical properties. B Stanly J.R., et. al. studied hybrid bamboo/glass woven fabrics in different orientations such as 0°/90° and ± 45°. The hybrid specimen with ±45° orientation yielded higher tensile strength and flexural strength when compared with 900 fiber orientation. Mohaiman J. Sharba, et. al. investigated the effect of fiber orientation on mechanical properties such as tensile strength, compression strength, and flexural strength of Glass/Kenaf hybrid composites. Results predicted that non-woven random mat Kenaf hybrid composite exhibited poor mechanical properties with other composite mats. P. Sathish, et.al. studied the effect of fiber orientation and stacking sequence on mechanical characteristics of banana/kenaf hybrid epoxy composites. The results showed that the hybrid composite with 450 fiber orientation had better properties than the other orientations. Mahmud Zuhudi, et.al. evaluated the mechanical, thermal and impact performances of the bamboo fabric-reinforced polymer composites. The results significant at the 50 wt.% of bamboo contents, where the tensile strength and its modulus were increased 238% and 100% compared to neat PP, respectively. Similarly, the flexural strength and modulus contributed to about at least 170% increase over the neat polypropylene.
Against this background, the present investigation has been undertaken to study of the mechanical behavior of bi-directional Bamboo and E-Glass fiber reinforced hybrid epoxy composites and compare with different fiber orientations.
II. MATERIALS AND METHODS A. Materials
In the present investigation, bi-directional E-Glass fiber was supplied by the Vijay trading corporation, J.C. Road, Bengaluru, India. Woven Bamboo fiber was procured from Jolly Enterprise, Kolkata, West Bengal (India).
Figure1 Bi-directional Bamboo and Glass fiber mat
curing, medium viscosity epoxy resin HSC 7600 and the hardener used was HSC 8210. Both resin and hardener procured from the Hindusthan Urban Infrastructure Ltd. (HUIL), Kolkata, West Bengal (India).
B. Preparation of composite laminates
Fabrication of the composite laminates was done by usual conventional hand lay-up technique followed by light compression molding technique. The mould was prepared with mild steel of size 310*310 mm2. It contains of two mild steel plates, lower die with rectangular slot and upper die with flat surface. Initially the mould was thoroughly cleaned by thinner solution and then coated with release agent used to facilitate easy removal of the composite from the mould. The mould was allowed to dry for 25 minutes. The composite laminate consists of seven layers of glass and six layers of bamboo fibers were placed alternately until the desired thickness might achieved. Woven bamboo fibers and glass fibers were arranged in three different orientations, namely 150, 30 0, and 600 with respective to the base fiber. The laminates were prepared from bamboo and glass fabrics of particular dimension 300*300*5 mm3. The laminates were named C1, C2, and C3 according to the various combinations of composites as mentioned in the Table 1. The epoxy resin was mixed with hardener in the proportion of 10:1 as recommended by manufacturer and then poured onto each layer of woven fabric and remove entrapped air bubbles if present. Both lower and upper dies were tightened with C-Clamps. Curing was done at room temperature for approximately 30 hours. As soon as the curing was completed, mould was opened and the laminate was taken out carefully . The same procedure was repeatedly followed to make other composite laminates as per different fiber orientations.
Table 1 Designation of laminates
Composite Fiber Orientation Fiber Content No. of Layers
Bamboo Glass Glass Bamboo
C1 50 50 7 6
C2 300 50 50 7 6
C3 600 50 50 7 6
C. Mechanical Properties of Composites
Tensile test: Rectangular shaped specimens were cut from the composite laminates with a length
250mm, width 25 mm using the power hacksaw machine and the edges were smoothed and finished to the required dimensions. All specimens were equipped with 50 mm long and 3 mm thick aluminum end-tabs, leaving specimen gauge length of 150 mm. Tensile tests were conducted according to ASTM-D3039 standard testing procedure using a computerized Universal Testing Machine. Specimens were placed in the grips and pulled at a constant strain rate of 3 mm/min until failure occurred.
Flexural test: This test is performed using 3-point bending test on rectangular specimens according
into ASTM-D790. Specimens were cut from the composite laminates with a length 127 mm and width 12.7 mm using the power hacksaw machine. The specimens were tested with a crosshead speed of 5 mm/min. The edges were smoothed and finished to the required dimensions of both tensile and flexural test specimens. Five specimens of each composite were tested for accuracy and then mean of the tensile strength and flexural strength was reported. The flexural strength (σ) was determined by using the following equation,
σ = 3PL (1)
Inter-Laminar Shear Strength (ILSS): It is also evaluated to help of data recorded during 3-point
bend test as per ASTM 2344 and ILSS is determined by using the following equation, ILSS= 3P (2)
Where, P is the maximum load in N, L is the span length of the sample in mm, w is the width of the specimen in mm, t is the thickness of the specimen in mm.
III. RESULTS AND DISCUSSION
Table 2 Mechanical properties of Bamboo-Glass hybrid epoxy composite laminates
Composite Fiber Tensile Tensile Flexural ILSS
Type Orientation Strength (MPa) Modulus (GPa) Strength (MPa) (MPa)
C1 150 97.2 2.49 207.95 5.59 C2 300 81.8 1.74 266.93 8.49 C3 600 75.8 2.04 210.12 6.43
A. Effect of Fiber Orientation on Tensile test
Different composite specimens are tested in the universal testing machine to determine the tensile properties. Figure 2 describes load v/s elongation curve obtained during a tensile test. The load can increases with respect to increase in elongation for the composites. The composite with 150 fiber orientation withstand a maximum load of 11.6 kN and maximum elongation of 7.9 mm and 300 fiber orientation withstand a maximum load of 11.06 kN. Similarly, 600 composite laminate shows a maximum load of 10.99 kN and maximum elongation of 8.8 mm. Composite type C1 can withstand more load than 600 specimen, but this composite type can exhibit more elongation than composite with 150 fiber orientation.
-1 0 1 2 3 4 5 6 7 8 9
The variation of tensile strength and tensile modulus of bamboo-glass hybrid fiber reinforced epoxy composites with different fiber orientations were presented in Figure 3 and 4. The tensile modulus is calculated by taking the corresponding values of stress and strain from the linear portion of the graph. The maximum tensile strength of composite was observed in 150 and minimum in 600 fiber orientation. Similarly, the maximum tensile modulus of composites was observed in 150 fiber orientation, which has a value 2.49 GPa and 300 fiber orientation exhibited 1.74 GPa lesser than other fiber orientations.
Figure 3 Tensile strength of bamboo-glass hybrid epoxy composites
Figure 4 Tensile modulus of bamboo-glass hybrid epoxy composites
B. Effect of Fiber Orientation on Flexural test
0 600 Orientation
-1 0 1 2 3 4 5 6 7 8 9
Figure 5 Load v/s displacement curve of bamboo-glass hybrid epoxy composites
Figure 6 Flexural strength of bamboo-glass hybrid epoxy composites
The maximum flexural strength of 266.93 MPa has been observed in 300 fiber orientation, 150 fiber orientation showed a flexural strength of 207.95 MPa, and 600 composite specimen show a value of flexural strength of 210.12 MPa. The results indicated that the composite with 300 fiber orientation shows better flexural strength than the 150 fiber orientation composite laminates tested.
C. Effect of Fiber Orientation on ILSS
Figure 7 ILSS of bamboo-glass hybrid epoxy composites
3.5 Surface Morphology
The failure morphological analysis of the tensile tested specimen is carried out using a scanning electron microscope (SEM). A sample specimen from each tensile test is taken for carrying out surface morphological analysis. The SEM image of each tensile specimen shows the nature of adhesion between the resin and the fibers and also the nature of failure of specimens after each test. The adhesion between epoxy resin and the fiber is good in the beginning. But after the tensile load has been applied to the composite laminate, the fibers pull out which leads to fiber breakage as observed in Figure 8 (a-c).
Figure 8 (a) SEM image of 150 laminate;(b) SEM image of 300 laminate;(c) SEM image of 600 laminate
The fiber has cracked at different locations, which indicates that a certain amount of energy has been absorbed during pull-out of the fibers from the matrix. From the micrographs of SEM analysis, the morphological properties like fiber breakage, fiber pull-out, fractured edge of fiber, dislocation of fiber and the orientation of the fiber of each tensile tested specimen and matrix due to various mechanical loadings were studied.
Based on the study of the mechanical properties of different layered fiber orientation of bamboo and glass hybrid fiber reinforced epoxy composites, the following conclusions can be drawn:
1. The successful fabrication of bamboo-glass hybrid fiber reinforced epoxy hybrid composites with different fiber orientations are possible by simple hand lay-up technique.
3. This experimental investigation revealed that composite with 300 fiber orientation shows a superior flexural strength than remaining fiber orientations
4. Composite laminate with 300 fiber orientation obtained maximum inter-laminar shear strength than when compared with remaining fiber orientations.
5.The effects of fiber orientation are analyzed and surface morphologies of composite laminates are studied using SEM and it is concluded that fiber orientation influences the mechanical behavior of the composite. SEM images of tensile tests identify fiber pull out from the composite laminate and fiber breakage during continuous loading conditions which is used to predict crack propagation in the composite.
This work can be further extended by introducing any filler materials in the epoxy matrix and also using various bio-degradable resins. Instead of the hand lay-up technique, other manufacturing techniques may be adopted to improve the mechanical properties of the composites.
Wambua P, Ivens J, Verpoest I., Natural fibres: can they replace glass in fibre reinforced plastics? Composite Science Technology 2003; 63, pp.1259-1264.
John K, and Venkata Naidu S, Sisal fibre/glass fibre hybrid composites: impact and compressive properties, Journal of Reinforced Plastic Composites 2004; 23(12), pp.1253-1258.
Murali Mohan Rao K, Mohana Rao K, Ratna Prasad AV, Fabrication and testing of natural fibre composites: Vakka, sisal, bamboo and banana, Mater Des 2010;31, pp.508-513.
R. Bhoopathi, M. Ramesh, C. Deepa, Fabrication and property evaluation of Banana-Hemp-Glass fiber reinforced composites, Procedia Engineering 97;2014, pp.2032-2041.
Soma Dalbehera, S. K. Acharya, Study on mechanical properties of natural fiber reinforced woven jute-glass hybrid epoxy composites, Advances in Polymer Science & Technology 2014;4(1), pp.1-6.
Byoung-Ho Lee, Hyun-Joong Kim, and Woong-Ryeol Yu. “Fabrication of Long and Discontinuous Natural Fiber Reinforced
Polypropylene Biocomposites and Their Mechanical Properties”. Fibers and Polymers 2009, Vol.10, No.1, pp. 83-90.
S. Jayabal, U Natarajan, M. Murugan, Mechanical property evaluation of woven coir and woven coir-glass fiber reinforced polyester composites, Journal of Composite Materials;2011 DOI: 10.1177/0021998311401080.
P. Sneha Latha, M. Venkateswara Rao, V.V. Kiran Kumar, G. Raghavendra, S. Ojha, Ramu inala, Evaluation of mechanical and tribological properties of bamboo-glass hybrid fiber reinforced polymer composite, Journal of Industrial Textiles 2015;DOI:10.1177/1528083715569376.
D. Dash, S. Samanta, S.S. Gautam, and M. Murlidhar, “Mechanical Characterizations of Natural Fiber Reinforced Composite Materials”, Advanced Materials Manufacturing & Characterization, Vol. 3, Issue 1, 2013, pp.275-279.
S. Biswas, Basu Deo, Amar Patnaik, Alok Satapathy, Effect of fiber loading and orientation on mechanical and erosion wear behaviors of Glass–Epoxy composites, polymer composites 2011; DOI:10.1002/pc.21082.
Vijaya Ramnath B, Santhosh Kumar V, Nirmal PV, Karthick S, Prem Kumar G, Elanchezhian C, Rajesh S, Suresh K., Experimental investigation of mechanical behavior of jute-flax based glass fiber reinforced composite, Fibers Polym 2014;15:1251-1262.
B Stanly Jones Retnam, M Sivapragash, P Pradeep, Effects of fiber orientation on mechanical properties of hybrid bamboo/glass fibre polymer composites, Indian Academy of Sciences 2014;37(5):1059-1064. Mohaiman J. S., Zulkiflle Leman, M.T.H. Sultan, Mohamad R. Ishak, Mohd. A.A. Hanim, Effects of
Kenaf fiber orientation on mechanical properties and fatigue life of Glass/Kenaf hybrid composites, Bio-Resources 2016;11(1):1448-1465.
P. Sathish, R. Kesavan, B. Vijaya Ramnath, C. Vishal, Effect of fiber orientation and stacking sequence on mechanical and thermal characteristics of Banana-Kenaf hybrid epoxy composite, 2014;DOI:10.1007/s12633-015-9314-7.
N.Z. Mahmud Zuhudi, K. Jayaraman1 and R.J.T. Lin, “Mechanical, Thermal and Instrumented Impact Properties of Bamboo Fabric-
Reinforced Polypropylene Composites”, Polymers & Polymer Composites, Vol. 24, No. 9, 2016, pp.755-766.